Books in black and white
 Books Biology Business Chemistry Computers Culture Economics Fiction Games Guide History Management Mathematical Medicine Mental Fitnes Physics Psychology Scince Sport Technics

# Polymer Chemistry. The Basic Concepts - Himenz P.C.

Himenz P.C. Polymer Chemistry. The Basic Concepts - Copyright, 1984. - 736 p.
Previous << 1 .. 156 157 158 159 160 161 < 162 > 163 164 165 166 167 168 .. 312 >> Next

we write
2fkd[l] = 2kt[M*]s2
(6.22)
Termination
363
or
/ f ê V/2
lM',s = \ir) [I1*
(623)
This important equation shows that the stationary-state free-radical
concentration increases with [I]1/2 and varies directly
with kd1/2 and inversely with ê{1/2.
The concentration of free radicals determines the rate at which polymer
forms and the eventual molecular weight of the polymer, since each
radical is a growth site. We shall examine these aspects of Eq. (6.23) in
the next section. We conclude this section with a numerical example which
concerns the stationary-state radical concentration for a typical system.
Example 6.2
For an initiator concentration which is constant at [I]0, the non-
stationary-state radical concentration varies with time according to the
following expression:
[M-] = exp[(16fkdkt[I]0)1/2t] - 1
[M ] s exp[(16fkdkc [I]0)1/2t] + 1
Calculate [M-]s and the time required for the free-radical concentration
to reach 99% of this value using the following as typical values for
constants and concentrations: kd = 1.0 X 10~4 sec"1, kt = 3 X 107 liter
mol"1 sec"1, f = lA, and [I] î = 10~3 M. Comment on the assumption [I] =
[I]0 that is made in deriving the non-stationary-state equation.
Solution
Use Eq. (6.23) to evaluate [M-]s for the system under consideration:
/fkd \1/2 /ÑË)(1.0Õ 10~4)(10"3) \1/2
[ì']' = Kl,4 -( .................Ø"' ) ¦ 0-"x .o-V
= 4.08 X 10"8 mol liter"1
This low level of concentration is typical of free-radical
polymerizations. Next we inquire how long it will take the free-radical
concentration to reach
0.99[M-]S, or 4.04 X 10~8 mol liter-1 in this case. Let a = (16fkdkt [I]
0)1/2 and rearrange the expression given to solve for t when [M ] / [M •]
s = 0.99:
0.99(eat + 1) = eat - 1, or 1 + 0.99 = eat(l - 0.99). Therefore the
product at = ln(l .99/0.01) = In 199 = 5.29, and a = [16(^)(1.0 X 10"4)(3
X 107) (10"3)]1/2 = 4.90 sec"1. Hence t = 5.29/4.90 = 1.08 sec. This
short period is also typical of the time required to reach the stationary
state.
364
The assumption that [I] = [I]0 may be assessed by examining the
integrated form of Eq. (6.2) for this system and calculating the ratio
[I]/[I]0 after 1.08 sec:
In | JjyLj = -kdt = -(1.0 X 10~4)(1.08) = -1.08 X 10~4
-Ô- = 0.99989
[I] î
Over the time required to reach the stationary state, the initiator
concentration is essentially unchanged. As a matter of fact, it would
take about 100 sec for [I] to reach 0.99[I]0 and about 8.5 min to reach
0.95[I]0, so the assumption that [I] = Øî is entirely justified over the
short time involved.
6.5 Propagation
The propagation of polymer chains is easy to consider under stationary-
state conditions. As the preceding example illustrates, the stationary
state is reached very rapidly, so we lose only a brief period at the
start of the reaction by restricting ourselves to the stationary state.
Of course, the stationary-state approximation breaks down at the end of
the reaction also, when the radical concentration drops toward zero. We
shall restrict our attention to relatively low conversion to polymer,
however, to avoid the complications of the Tromms-dorff effect. Therefore
deviations from the stationary state at long times need not concern us.
Consideration of reaction (6.B) leads to
= kptMHM]
(6.24)
as the expression for the rate at which monomer is converted to polymer.
In writing this expression, we assume the following:
1. The radical concentration has the stationary-stage value given by
Eq. (6.23).
2. kp is a constant independent of the size of the growing chain and
the extent
of conversion to polymer.
3. The rate at which monomer is consumed is equal to the rate of polymer
formation Rp:
-d[M] = d[polymer] _ R
^ 25)
Propagation
365
Combining Eqs. (6.23) and (6.24) yields
_ _ 1A . .,
Rp = kp[M] ,/* = êàðð[Ì][1]é
(6.26)
in which the second form reminds us that an experimental study of the
rate of polymerization yields a single constant (subscript app) which the
mechanism reveals to be a composite of three different rate constants.
Equation (6.26) shows that the rate of polymerization is first order in
monomer and half order in initiator and depends on the rate constants for
each of the three types of steps-initiation, propagation, and
termination-that make up the chain mechanism. Since the concentrations
change with time, it is important to realize that Eq. (6.26) gives an
instantaneous rate of polymerization at the concentrations considered.
Previous << 1 .. 156 157 158 159 160 161 < 162 > 163 164 165 166 167 168 .. 312 >> Next